Successfully reported this slideshow.
Module-I of Manufacturing Science-I 1.4 MOULDING MATERIAL AND PROPERTIES A large variety of molding materials is used in foundries for manufacturing molds and cores. Theyinclude molding sand, system sand or backing sand, facing sand, parting sand, and core sand. The choice ofmolding materials is based on their processing properties. The properties that are generally required inmolding materials are:RefractorinessIt is the ability of the molding material to resist the temperature of the liquid metal to be poured so that itdoes not get fused with the metal. The refractoriness of the silica sand is highest.PermeabilityDuring pouring and subsequent solidification of a casting, a large amount of gases and steam is generated.These gases are those that have been absorbed by the metal during melting, air absorbed from theatmosphere and the steam generated by the molding and core sand. If these gases are not allowed to escapefrom the mold, they would be entrapped inside the casting and cause casting defects. To overcome thisproblem the molding material must be porous. Proper venting of the mold also helps in escaping the gasesthat are generated inside the mold cavity.Green StrengthThe molding sand that contains moisture is termed as green sand. The green sand particles must have theability to cling to each other to impart sufficient strength to the mold. The green sand must have enoughstrength so that the constructed mold retains its shape.Dry StrengthWhen the molten metal is poured in the mold, the sand around the mold cavity is quickly converted into drysand as the moisture in the sand evaporates due to the heat of the molten metal. At this stage the moldingsand must posses the sufficient strength to retain the exact shape of the mold cavity and at the same time itmust be able to withstand the metallostatic pressure of the liquid material.Hot StrengthAs soon as the moisture is eliminated, the sand would reach at a high temperature when the metal in themold is still in liquid state. The strength of the sand that is required to hold the shape of the cavity is calledhot strength.CollapsibilityThe molding sand should also have collapsibility so that during the contraction of the solidified casting itdoes not provide any resistance, which may result in cracks in the castings. Besides these specificproperties the molding material should be cheap, reusable and should have good thermal conductivity.TESTING SAND PROPERTIES The moulding sand after it is prepared, should be properly tested to see that the requisite propertiesare achieved. These are standard tests to be done as per Indian Standards.Sample PreparationTests are conducted on a sample of the standard sand. The moulding sand should be prepared exactly as isdone in the shop on the standard equipment and then carefully enclosed in a container to safeguard itsmoisture content.Moisture Content Moisture is an important element of the moulding sand as it affects many properties. To test themoisture of moulding sand a carefully weighed sand test sample of 50g is dried at a temperature of 1050 Cto 1100 C for 2 hours by which time all the moisture in the sand would have been evaporated. The sample isthen weighed. The weight difference in grams when multiplied by two would give the percentage ofmoisture contained in the moulding sand. Alternatively a moisture teller can also be used for measuring themoisture content. In this sand is dried by suspending the sample on a fine metallic screen and allowing hotair to flow through the sample. This method of drying completes the removal of moisture in a matter ofminutes compared to 2 hours as in the earlier method. Another moisture teller utilizes calcium carbide to measure the moisture content. A measuredamount of calcium carbide ( a little more than actually required for complete reaction) in a container alongwith a separate cap consisting of measured quantity of moulding sand is kept in the moisture teller. Care Lecture Notes of Chinmay Das 21
Module-I of Manufacturing Science-Ihas to be taken before closing the apparatus that carbide and sand do not come into contact. The apparatusis then shaken vigorously such that the following reaction takes place: CaC2 + 2 H2O → C2H2 + Ca(OH)2The acetylene ( C2H2) coming out will be collected in the space above the sand raising the pressure. Apressure gauge connected to the apparatus would give directly the amount of acetylene generated which isproportional to the moisture present. It is possible to calibrate the pressure gauge directly read the amountof moisture.Clay Content The clay content of the moulding sand is determined by dissolving or washing it off the sand. Todetermine the clay percentage a 50 g sample is dried at 105 to 1100 C and the dried sample is taken in a onelitre glass flask and added with 475 ml of distilled water and 25ml of a one percent solution of caustic soda(NaOH 25 g per litre). This sample is thoroughly stirred. After the stirring, for a period of five minutes, the sample is diluted with fresh water up to a 150mm graduation mark and the sample is left undisturbed for 10 minutes to settle. The sand settles at thebottom and the clay particles washed from the sand would be floating in the water. 125 mm of this water issiphoned off the flask and it is again topped to the same level and allowed to settle for five minutes. Theabove operation is repeated till the water above the sand becomes clear, which is an indication that all theclay in the moulding sand has been removed. Now, the sand removed from the flask and dried by heating.The difference in weight of the dried sand and 50g when multiplied by two gives the clay percentage in themoulding sand.Sand Grain Size To find out the sand grain size, a sand sample which is devoid of moisture and clay such as theone obtained after the previous testing is to be used. The dried clay free sand grains are placed on the topsieve of a sieve shaker which contains a series of sieves one upon the other with gradually decreasing meshsizes. The sieves are shaken continuously for a period of 15 minutes. After this shaking operation, thesieves are taken apart and the sand left over on each of the sieve is carefully weighed. The sand retained oneach sieve expressed as a percentage of the total mass can be plotted against sieve number. But moreimportant is the Grain Finesses Number (GFN) which is a quantitative indication of the grain distribution.To calculate the GFN each sieve has been given a weightage factor as given in the Table –IV. The amountretained on each sieve is multiplied by the respective weightage factor, summed up and then divided by thetotal mass of the sample, which gives the GFN. Figure 1.4.1: Sieve shaker Lecture Notes of Chinmay Das 22
Module-I of Manufacturing Science-I Mathematically GFN = ∑Mf i i ∑f iWhere Mi = multiplying factor for the ith sieve fi = amount of sand retained on the ith sieve US Series Equivalent No. IS Sieve No. Mesh Opening(mm) Multiplying Factor (ASTM) Microns 6 3.327 3.35 3 12 1.651 1.70 5 20 0.833 850 10 30 0.589 600 20 40 0.414 425 30 50 0.295 300 40 70 0.208 212 50 100 0.147 150 70 140 0.104 106 100 200 0.074 75 145 270 0.053 53 200 PAN - - 300 Table-IV: AFS Sieve Numbers and Their Indian Equivalents with sizesA typical example is presented in Table-V for calculation of GFN. Retained Multiplying RetainedSieve Number Percentage Mi x Pi Mi x fi Factor, Mi Sample, fi (g) Pi 40 30 2.495 5 150 74.85 50 40 13.972 28 1120 558.88 70 50 23.952 48 2400 1197.60 100 70 6.986 14 980 489.02 140 100 2.495 5 500 249.50 49.900 100 5150 2569.85 Table-V Mi x Pi 5150GFN = = = 51.50 Pi 100 Mi x fi 2569.85 = = = 51.50 fi 49.90GFN is the average grain size and corresponds to a sieve number through which all the sand grains wouldpass through, if they were all of the same size. GFN value varies between 40 and 220 for those sands usedby most of the foundries. Though the sand properties depend on both the grain size and the grain sizedistribution, GFN is a very convenient way of finding the sand properties since it takes both into account.Example: GFN 41 : steel castings 50 Kg and more 67 : Small steel castings 105: Light cast iron and copper castings 150: Aluminium alloy castings Lecture Notes of Chinmay Das 23
Module-I of Manufacturing Science-IPermeabilityThe rate of flow of air passing through a standard specimen under a standard pressure is termed aspermeability number. The standard permeability test is to measure time taken by a 2000 cm3 of air at apressure typically of 980 Pa to pass through a standard sand specimen confined in a specimen tube. Thestandard specimen size is 50.8 mm in diameter and a length of 50.8 mm. Then, the permeability number, Pis obtained by VXH P= pxAxTWhere V = volume of air = 2000 cm3 H = height of the sand specimen = 5.08 cm p = air pressure, g/cm2 A = cross sectional area of sand specimen= 20.268 cm2 T = time in minutes for the complete air to pas throughInserting the above standard values into the expression, we get 501.28 P= p.T Figure 1.4.2: Permeability measuring set upSpecimen PreparationSince the permeability of sand is dependent to a great extent, on the degree of ramming, it is necessary thatthe specimen be prepared under standard conditions. To get reproducible ramming conditions, a laboratorysand rammer is used along with a specimen tube. The measured amount of sand is filled in the specimentube, and a fixed weight of 6.35 to 7.25 Kg is allowed to fall on the sand three times from a height of 50.8 ±0.125 mm. The specimen thus produced should have a height of 50.8± 0.8 mm. To produce this size ofspecimen usually sand of 145 to 175 g would be required. After preparing a test sample of sand asdescribed, 2000 cm3 of air are passed through the sample and time taken by it to completely pass throughthe specimen is noted. Lecture Notes of Chinmay Das 24
Module-I of Manufacturing Science-I Figure 1.4.3: Sand rammer for specimen preparationStrengthMeasurement of strength of moulding sands can be carried out on the universal sand strength testingmachine. The strength can be measured in compression, shear and tension. The sands that could be testedare green sand, dry sand or core sand. The compression and shear test involve the standard cylindricalspecimen that was used for the permeability test.Green Compression StrengthGreen compression strength or simply green strength generally refers to the stress required to rupture thesand specimen under compressive loading. The sand specimen is taken out of the specimen tube and isimmediately (any delay causes the drying of the sample which increases the strength) put on the strengthtesting machine and the force required to cause the compression failure is determined. The green strengthof sands is generally in the range of 30 to 160 KPa.Green Shear StrengthWith a sand sample similar to the above test, a different adapter is fitted in the universal machine so that theloading now be made for the shearing of the sand sample. The stress required to shear the specimen alongthe axis is then represented as the green shear strength. It may vary from 10 to 50 KPa.Dry Strength This test uses the standard specimens dried between 105 and 1100 C for 2 hours. Since the strengthincreases with drying, it may be necessary to apply larger stresses than the previous tests. The range of drycompression strengths found in moulding sands is from 140 to 1800 KPa, depending on the sand sample. Figure 1.4.4: Sand strength testing set up Lecture Notes of Chinmay Das 25
Module-I of Manufacturing Science-I Figure 1.4.5: Universal sand strength measuring set upMould HardnessThe mould hardness is measured by a method similar to the Brinell hardness test. A spring loaded steel ballwith a mass of 0.9 Kg is indented into the standard sand specimen prepared. The depth of indentation canbe directly measured on the scale which shows units 0 to 100. When no penetration occurs, then it is amould hardness of 100 and when it sinks completely, the reading is zero indicating a very soft mould. Figure 1.4.6: Mould and core hardness tester Besides these, there are other tests to determine such properties as deformation, green tensilestrength, hot strength, expansion, etc.Reference:1. Manufacturing Technology by P.N.Rao, TMH Lecture Notes of Chinmay Das 26